Successfully reported this slideshow.
Upcoming SlideShare
×

# Galvanizing Inspection of Structure

4,225 views

Published on

Published in: Engineering
• Full Name
Comment goes here.

Are you sure you want to Yes No
• Dating direct: ♥♥♥ http://bit.ly/2Q98JRS ♥♥♥

Are you sure you want to  Yes  No
• Dating for everyone is here: ❤❤❤ http://bit.ly/2Q98JRS ❤❤❤

Are you sure you want to  Yes  No
• 8 Simple Tips &amp; Tricks To Extend The Life Of Your Car Battery.. ●●● https://bit.ly/2t1uc6e

Are you sure you want to  Yes  No
• I didn't think failing my maths back in high school would come back to haunt me but it did! After graduating from Edge Hill University, I was looking to undertake a PGCE in primary teaching. However, one of the requirements was a pass in GCSE maths so I had no choice but to re-take it. After failing it twice, my confidence was very low and I didn't think I could qualify for the PGCE. After running a Google search on passing GCSE maths, I came across Jeevan's revision system. The feedback it received looked very good so I decided to give it a try... And it was one of the best decisions I've ever made. After going through Jeevan's guide, I managed to grasp the entire subject and I passed my next GCSE maths exam, with ease. He (Jeevan) provided me with all the tools I needed to prepare for the exam. Together with his guidance, my pass was a foregone conclusion. Thank you so much Jeevan! You have potentially changed my life. I recommend anyone seeking a pass grade in GCSE maths to purchase this fantastic package!★★★ http://t.cn/AirraVnG

Are you sure you want to  Yes  No
• Discover A Simple Holistic System For Curing Acne Once And For All using 100% Guaranteed All-Natural Method. Click Here ♥♥♥ https://tinyurl.com/ybbtmvh8

Are you sure you want to  Yes  No

### Galvanizing Inspection of Structure

1. 1. HOT DIP GALVANIZERS ASSOCIATION SOUTHERN AFRICA The Association is a technical information centre established for the benefit of specifiers, consultants, end users and its members PRACTICAL GUIDELINES FOR THE INSPECTION AND REPAIR OF HOT DIP GALVANIZED COATINGS
2. 2. HOT DIP GALVANIZERS ASSOCIATION SOUTHERN AFRICA Quality House, St. Christopher Road, St. Andrews, Bedfordview P O Box 2212, Edenvale, 1610 Telephone: (011) 456-7960 Fax: (011) 454-6304 Email: hdgasa@icon.co.za www.hdgasa.org.za The Association is a technical information centre established for the benefit of specifiers, consultants, end users and its members The copyright of all material in this catalogue and its supplements, particularly material which is identified by the symbol ©, is expressly reserved. No part of this catalogue may be reproduced or distributed in any form or by any means, without the prior written permission of Hot Dip Galvanizers Association South Africa. Whilst every effort has been made to ensure the accuracy of the information contained in this publication, no responsibility can be accepted for any errors or for any direct or consequential loss or damage resulting from such information.
3. 3. Foreword “Practical Guidelines for the Inspection and Repair of Hot Dip Galvanized Coatings”, has been compiled with reference to the new international specifications. These include: SANS 121 / ISO 1461 Hot dip galvanized coatings on fabricated iron and steel articles – Specifications and test methods. SANS 32 / EN 10240 Internal and/or external protective coatings for steel tubes– Specification for hot dip galvanized coatings applied in automatic plants. SANS 14713 / ISO 14713 Protection against corrosion of iron and steel in structures – Zinc and aluminium coatings – Guidelines. Although specifications SABS 763 and SABS 0214 have been replaced, for practical reasons reference has also been made to: SABS 763 Hot-dip (galvanized) zinc coatings (other than on continuously zinc coated sheet and wire). The guidelines take into account recognised engineering principles, inspection practices and practical experience accumulated over the years by the Hot Dip Galvanizers Association of Southern Africa established in 1965. The guidelines have been formulated for general information only and although practically enforceable, they are not intended as a substitute for competent professional examination and verification as to accuracy, suitability and/or applicability, by a trained HDGASA inspector. The publication of the material contained in this booklet is not intended as a representation or warranty on the part of the Hot Dip Galvanizers Association of Southern Africa. Anyone making use of this information assumes all liability arising from such use. Due to the frequent use of misleading terms such as “cold galvanizing” to describe zinc rich paint and electrogalvanizing for zinc electroplating, the specifier who requires hot dip galvanizing for corrosion control, should specify that all components shall be hot dip galvanized in accordance with the requirements of SANS 121 / ISO 1461 or SANS 32 / EN 10240 as applicable. HDGASA © 2005 1
4. 4. HDGASA © 2005 Contents Introduction .................................................................................... 3 Test Sampling.................................................................................. 3 Thickness and Uniformity ................................................................ 3 Thickness Testing ............................................................................ 5 Surface Conditions – Acceptance, Rejection and Responsibility ...... 8 Reference areas .............................................................................. 15 Uniformity Testing .......................................................................... 15 Adherence of the Coating .............................................................. 16 Testing Adherence .......................................................................... 16 Appearance .................................................................................... 16 Removal of Wet Storage Stain (White Rust) .................................... 17 Coating Repair Procedures – By the Galvanizer ............................ 17 – Site Repairs ...................................... 18 Applicable Standards ...................................................................... 19 Aims and Objectives of the Association .......................................... 20 Publications Available from the Association .................................... 20 2
5. 5. Introduction Hot dip galvanizing is one of the most widely used methods of protecting steel from corrosion. As a final step in the process, the hot dip galvanized coating is inspected for compliance with specifications. Interpretation of inspection results should be made with a clear understanding of the causes of the various con-ditions which may be encoun-tered and their effects on the ulti-mate objective of providing cor-rosion protection. This manual has been designed to assist in testing, inspection, and the interpretation of test results. It deals with numerous surface con-ditions, their origins, and their effects on protection from corro-sion. This manual also considers undesirable design and fabricating features as well as unacceptable hot dip galvanizing practice. Although it is difficult to cover every condition, the manual cov-ers many of the conditions fre-quently encountered in practice. To effectively use this manual, inspectors should remember that the main purpose of hot dip gal-vanizing is to protect steel from corrosion. The length of time this protection can reasonably be expected to last is called its “ser-vice life or time to first mainte-nance”. This is defined as the time taken for the appearance on an article of 5% surface rust. The service life of a hot dip galva-nized coating is directly pro-portional to the thickness of the coating. Corrosion protec-tion is greater when the coat-ing is thicker. Thus coating thickness is the single most important inspection check to determine the quality of a hot dip galvanized coating. Coating thickness, however, is only one inspection aspect. Other features include the uni-formity of the coating, coating adhesion and appearance. Possible brittleness and de-fects, which arise from incor-rect design and fabrication, also need to be assessed by the inspectorate. While minimum specified stan-dards must be satisfied, their rel-ative importance varies accord-ing to the end use of the prod-uct. For example, the aesthetic appearance of hot dip galvanized structural steel in an obscured application is different from that where a product is used as an architectural feature. An aware-ness of the end use of the prod-uct and the capability of the hot dip galvanizing process is essen-tial for good inspection. Inspection of hot dip galvanized products, as the final step in the process, can be most effectively and efficiently conducted at the galvanizer’s plant. Here, ques-tions can be raised and answered quickly, inspection speeded up and, the time saved is beneficial. Occasionally, due to rough han-dling and possible site modifica-tions, which include cutting and welding, coating repairs become necessary. Repair procedures and the recommended repair materi-als are covered in this manual. The quality standards to which ref-erence is made in the following sections are in accordance with International and South African National Standards’ specifications. Test Sample Selection To effectively evaluate hot dip gal-vanized coatings, it is essential that randomly selected specimens be representative of an inspection lot. An inspection lot is a single order or batch awaiting despatch. For products required to comply with SANS 121 / ISO 1461 the minimum number of articles from each inspection lot that forms the control sample shall be in accor-dance with table 1 of the specifi-cation. Typically, the test unit for compli-ance with SANS 32 / EN 10240 shall be, for each size, one tube per first 500 tubes and subse-quently one per 1000 tubes for outside diameters greater than 21.3mm and one per 2000 tubes for smaller diameters. Unless otherwise specified by the purchaser, an acceptance inspec-tion should be arranged and undertaken before the products leave the premises of the galva-nizer. Coating Thickness and Uniformity The thickness of the hot dip gal-vanized coating is the primary factor in determining its life under given service conditions. The thicker the coating, the bet-ter corrosion protection it offers. For most atmospheric conditions, HDGASA © 2005 3 TABLE 1 Number of articles in the lot Minimum number of articles in the control sample 1 to 3 All 4 to 500 3 501 to 1200 5 1201 to 3200 8 3201 to 10 000 13 > 10 000 20
6. 6. the relationship between corro-sion protection and coating thick-ness is approximately linear, i.e., the service life is doubled if the coating thickness is doubled. There is however a limit to the maximum coating thickness that can be obtained. The factors which influence over-all coating thickness are a combi-nation of several variables. The galvanizer can alter zinc temper-ature, time of immersion and rate of withdrawal from the molten zinc. These factors can be used to marginally alter coating thick-ness, particularly with reactive steels. The formation of the pro-tective iron/zinc alloy layer is a diffusion process. As with all dif-fusion processes, the reaction proceeds rapidly at first and slows down as the layer becomes thicker. Higher bath temperatures and longer immersion times will generally produce thicker alloy layers. The thickness of the outer zinc layer of the coating is indepen-dent of immersion time. Thickness of this layer is deter-mined by the rate of withdrawal from the zinc bath and the degree of drain-off of molten zinc. A fast rate of withdrawal causes an article to “drag out” more zinc. This results in a heav-ier coating, although the distribu-tion of the zinc layer may be uneven. Wiping of the coating during withdrawal materially reduces its thickness and thus its protective value. It is discour-aged except where necessary for the smoothness demanded by conditions of service such as for small bore pipe and conduit. Tubes hot dip galvanized in accordance with SANS 32 / EN 10240 utilise steam blowing internally and an air ring exter-nally, to remove excess zinc. Some variation in internal coat-ing thickness is acceptable within 50mm of tube ends. With fabri-cated articles, local differences in the drain-off, because of the shape of the article and the angle at which different surfaces leave the bath, may also result in some variation in coating thickness. Other factors influencing the coating thickness may be beyond the control of the galva-nizer. The chemical composition of the steel plays a major role in deter-mining the thickness and appearance of the final coating. Certain steel compositions tend to accelerate the growth of the iron/zinc alloy layer so that the hot dip galvanized coating may have a matte finish with little or no outer zinc layer. This coating also tends to be thicker than the typical bright hot dip galvanized coating. The galvanizer’s control over this condition is limited. Steels containing the elements, phosphorus in excess of 0.03%, or silicon from 0.05% to 0.12% and above 0.3% or combinations of both elements, are particularly prone to heavier coatings con-sisting mainly of iron/zinc alloys. Due to the iron/zinc alloy growth in these coatings, extending to the outer surface, the final appearance of the coat-ing can be dark grey in colour distributed evenly or unevenly over the surface. The surface condition of the steel before hot dip galvanizing also affects the thickness and smoothness of the final coating. Steels which have been abrasive blast cleaned, or left to weather and rust for some time prior to hot dip galvanizing, can produce substantially thicker coatings than those normally produced on chemically cleaned steel. The mass, shape and degree of cold working of components to be hot dip galvanized also influences coating thickness and uniformity. When a fabricated article consists of both heavy and light sections, a TABLE 2 MINIMUM COATING THICKNESS ON ARTICLES THAT ARE NOT CENTRIFUGED SANS 121 / ISO 1461 SABS 763 Category and Local Mean Article Thickness, thickness coating coating Type μm. (t) mm thickness thickness General μm* μm* Application t ≥ 6 70 85 A1, B1, D1, 85 E1, F1 3 ≤ t < 6 55 70 A2, B2, F2 65 1.5 ≤ t < 3 45 55 t < 1.5 35 45 A3 45 B3 55 F3 45 t ≥ 6 70 80 D1 85 t < 6 60 70 * Local coating thickness is defined as the mean of the measurements taken within a specified reference area. Mean coating thickness is the control sample number average of the local coating thickness values from each reference area. Thickness legend - 3 ≤ t 6 = thickness less than 6mm but greater and equal to 4 HDGASA © 2005 3mm. Where only one reference area is required according to size of the article, the mean coating thickness within that reference area shall be equal to the mean coating thickness given in the above table. CASTINGS PROFILES
7. 7. variation in coating thickness between the sections may result. Immersion time will vary accord-ing to the relationship of the sur-face area of an item to its mass. The galvanizer has little control over this situation. Combining heavy and light sec-tions in a single component may also result in unacceptable distor-tion (refer to HDGASA wall chart, “Design for Hot Dip Galvanizing”). Since the time to the appearance of first rusting of the base steel is usually determined by the thinnest portion of the coating, an evaluation of galvanizing qual-ity must take into account both the minimum thickness of the coating and its distribution. Specifications for hot dip galva-nizing recognise that variations in coating thickness are inherent in the process. The minimum thick-ness is generally defined as an average or mean thickness of the coating on specimens tested and/or a minimum thickness for any individual specimen. When measurements are taken to determine the uniformity and thickness of a hot dip galvanized coating, 5 or more coating thick-ness readings should be taken in each reference area. Reference areas should be taken approxi-mately 100mm from the ends of the article to avoid end effects. Usually the end of an article which leaves the bath last will carry a thicker coating. This is particularly so towards the edge, where, at the time of drainage, the last few drops of zinc tend to agglomerate as a result of sur-face tension. The minimum coating require-ments specified in SANS 121 / ISO 1461 for different material thicknesses and classes of work are summarized in table 2 and table 3. For comparitive purpos-es, these tables compare thick-ness equivalents to the old SABS 763 specification. Table 4 indi-cates the minimum coating requirements specified in SANS 32 / EN 10240 for different classes of coating. Specifications do not stipulate maximum upper coating thick-ness limits, but excessively thick coatings on threaded articles are undesirable. In order to ensure effective tensioning, the coating thickness on fasteners should not exceed a maximum of 65μm, this applies particu-larly, to high strength bolts and nuts. Variance in coating thickness. A requirement for a thicker coat-ing (25% greater than the stan-dard in table 2) can be request-ed for components not cen-trifuged, without affecting speci-fication conformity. NOTE: Where steel composition does not induce moderate to high reactivity, thicker coatings are not always easily achieved. Thicker coatings are more resis-tant to severe environmental conditions, but can be more brittle and may require special handling. The efficacy of corro-sion protection of a hot dip gal-vanized coating (whether light or dull grey) is approximately proportional to coating thick-ness. Thickness Testing There are several methods to determine the thickness of the zinc coating on a hot dip galva-nized article. The size, shape and number of pieces to be tested, will most likely dictate the meth-ods of testing. The specified test methods are either destructive or non-destructive and are detailed in SANS 121 / ISO 1461. Identical methods are detailed in SANS 32 / EN 10240. The most practical tests are the non-destructive type, such as gauges utilising the electromagnetic principle. 1. Electromagnetic Testing Method. Instruments, which rely on electromagnetic principles are probably the most widely HDGASA © 2005 5 TABLE 3 MINIMUM COATING THICKNESS ON ARTICLES THAT ARE CENTRIFUGED SANS 121 / ISO 1461 SABS 763 Category and Local Mean Article Thickness, thickness/diameter coating coating Type μm. (t) or (ø) mm thickness thickness General μm* μm* Application ø ≥ 20 45 55 C1 55 6 ≤ ø 20 35 45 C2 45 ø 6 20 25 t ≥ 3 45 55 C1 Washers 55 D2 45 t 3 35 45 C2 Washers 45 * Local coating thickness is defined as the mean of the measurements taken within a specified reference area. Mean coating thickness is the control sample number average of the local coating thickness values from each reference area. Thickness/diameter legend - 6 ≤ ø 20 = diameter less than 20mm but greater and equal to 6mm. Where only one reference area is required according to size of the article, the mean coating thickness within that reference area shall be equal to the mean coating thickness given in the above table. OTHER ARTICLES FASTENERS (INCLUDING CASTINGS)
8. 8. Capable of minimizing errors in reading caused by the magnetic perme-ability, dimensions, sur-face finish and curvature of the article being test-ed; Capable of measuring the thickness of the coating being tested within an accuracy of 10% or 1.5μm whichever is betterA, and Calibrated by taking readings at zero (or near zero) thickness and at thicknesses of at least 100μm, on suitable non-ferrous shims placed on acceptable standard pieces of metal of com-position, thickness and shape similar to those of the articles under test. To avoid possible errors in the use of magnetic instru-ments, certain precautions should be taken: Follow the manufacturer’s instructions. The instru-ment should be frequent-ly recalibrated against non-magnetic film stan-dards of known thick-ness. The base steel should be backed up with similar material if thinner than the critical thickness for the magnetic gauge or the instrument should be recalibrated on a sub-strate of similar thick-ness. Readings should not be taken near an edge, hole, or inside corner. HDGASA © 2005 used devices to determine the thickness of hot dip gal-vanized coatings. Electro-magnetic instruments mea-sure coating thickness in specifically-identified local areas of the article. The aver-age thickness (and therefore mass) of the coating is calcu-lated from measurements taken at a suitably large num-ber of points distributed over a reference area on the sur-face of the article. There are a number of electromagnetic gauges which can be used to give accurate measurements of the zinc coating thickness. These gauges give reliable thickness readings provided they are properly calibrated and the manufacturer’s instructions are observed. The most commonly used type of gauge is a portable electronic instrument. The gauge uses a temperature-compensated magnetic trans-ducer to measure the mag-netic flux changes that occur when the probe (a magnet) is separated from a ferrous metal substrate by a non-magnetic coating such as zinc. The output signal from the probe is propor-tional to the distance of separation and, therefore, to coating thickness. The probe signal is amplified and indicated on a meter calibrated to show coating thickness. These battery powered instruments have typical accuracies up to 5% and have the advantage of not requiring recalibration with probe orientation. Similar electromagnetic instruments with even greater accuracies are avail-able for laboratory use. The specification requires that the thickness gauges shall (in terms of ISO 2178) be - 6 TABLE 4 MINIMUM COATING THICKNESS ON STEEL TUBES TO SANS 32 / EN 10240 COATING QUALITY A1 A2 A3 Mandatory Minimum local coating thickness on the inside surface except at the weld bead 55μm 55μm 45μm Minimum local coating thickness on the inside surface at the weld bead 28μm 1) 1) Options Minimum local coating thickness on the outside surface 2) 2) 2) COATING QUALITY B1 B2 B3 Mandatory Minimum local coating thickness on the outside surface 55μm 3) 40μm 25μm 1) This requirement does not apply 2) This requirement applies when the purchaser specifies Option 1 3) Option 3 specified (if 55μm required, purchaser to specify according to SANS 121 / ISO 1461) Coating qualities ‘A’ and ‘B’ refer to end application with quality ‘A’ being for gas and water installations and ‘B’ for other applications. The number following the quality letter refers to specific requirements in terms of coating thickness. NOTE: In South Africa, SANS 32 / EN 10240 to quality A1 replaces the previous SABS 763, B4 coating. A When curved surfaces are dealt with, particular care should be taken to ensure that the thickness gauge is capable of obtaining readings to an acceptable level of accuracy.
10. 10. Surface Conditions (SC) LEGEND: A - Accept R - Reject N - Negotiate C - Clean REP - Repair RESPONSIBILITY: G - Galvanizer D - Designer B - Builder/Fabricator S - Steel Type/Surface SC DESCRIPTION CAUSE EFFECT / REMEDY A/R/N EXAMPLE RESPONSIBILITY C/REP AVAILABLE BATH 1 APPEARANCE OF A Although the recommended quantity of sodium dichromate is about 0,15 to 0,3%, occasionally when topping up, more is added. This often results in a dark yellow to brown colour on the galvanized surface. The darker colour will provide enhanced initial corrosion protection. SODIUM DICHROMATE. A small amount of sodium dichromate is generally added to the quench water bath for passivation. G Maintain concentration of sodium dichromate at about 0,15 to 0,3%. 2 ASH DEPOSITS A / N Ash deposits are grey, non-metallic deposits consisting of zinc oxide that have been deposited on the hot dip galvanized coating. C/REP G If necessary Zinc oxide deposits can take place when the component is dipped or when it is removed from the bath. The coating is normally intact underneath the ash deposits. Ash must be removed and the coating thickness verified for conformance to the specification requirements. Remove ash from all liquid conveyance pipes. 3 BARE SPOTS. A / R There are several causes of bare spots. These include: Overdrying. If the time between fluxing and hot dip galvanizing is prolonged or the drying temperature is too high, the barrier protection provided by the flux may be lost. This is indicated by a rusty appearance on the ungalvanized article, which can result in coating discontinuities after hot dip galvanizing. G Excess Aluminium. A condition sometimes referred to as black - spots may occur if the aluminium content of a bath becomes too high. No trouble should be experienced if flux concentration is correct and the aluminium content of the bath is maintained below approximately 0,007%. G Further causes are: Blowouts; flux deposits; stains and inclusions; mechanical damage; touch marks; uncoated surfaces caused by - surface contaminants, scale or sand; welds and weld spatter. See SC No’s 6, 16, 19, 30, 33, 34, 35 and 37 Although excluded from SANS 121 / ISO 1461, bare spots of about 5mm2 (2,2 x2,2mm), due to small localised flaws, are adequately protected by the sacrificial properties of zinc and will have very little effect on the service life of the coating. Where necessary, such spots may be repaired using one of the specified repair methods. Gross uncoated areas are a cause for rejec- REP tion. See Coating If Repair Procedures. necessary 4 BLACK STEEL A / R INSPECTION. Inspection prior to hot dip galvanizing is extremely important. Components should be checked for distortion caused during rolling or fabrication. Check for appropriate vent, fill and drainage holes: removal of weld slag and spatter; venting of overlapping surfaces; unsuitable joining materials; temporary identification markings; clearance for moving parts and potential distortion due to the process. Insufficient inspection prior to hot dip galvanizing can be the cause of dispute. G 8 HDGASA © 2005
11. 11. SC DESCRIPTION CAUSE EFFECT / REMEDY A/R/N EXAMPLE RESPONSIBILITY C/REP 5 BLASTING DAMAGE. R Sweep blasting, done correctly, substantially increases paint adhesion and final coating appearance but done incorrectly can result in coating damage. Incorrect nozzle pressure; nozzle angle; sweeping distance; size of abrasive and recycling of grit. A hot dip galvanized coating will be partially or fully destroyed by excessive blasting. Refer to the HDGASA Code of Practice. D/B 6 BLOWOUTS. A Staining and coating defects around unsealed weld areas and vent holes. Similar to stains caused by weeping . See SC 28. C / REP If necessary Pre-treatment chemicals penetrating sealed overlap areas through the required vent holes and escaping during immersion in the molten zinc. This effect tends to damage the flux coating, causing localised uncoated areas. Pre-heat item prior to immersion in zinc bath to dry out overlap area as much as possible. G/D 7 CLOGGED HOLES. A Zinc film clogging or partly bridging holes. C If required Molten zinc has a high surface tension and will not easily drain from holes under 8mm in diameter. Make holes as large as possible. Removal of molten zinc over the bath and utilization of vibrators will reduce the likelihood of clogging. D/G 8 CLOGGED THREADS. R Threaded components or attachments have threads clogged with zinc C / REP Insufficient centrifuging or poor drainage of threaded attachments on withdrawal from the galvanizing bath. The correct centrifuging equipment or post galvanizing thread cleaning by heating, wire brushing or oversize tapping of nuts, will generally remove clogging. If necessary specify delivery of bolts and nuts in nutted up form. G 9 DESIGN STRUCTURES A IN MODULAR LENGTHS AND OPTIMUM WIDTHS TO SUIT AVAILABLE BATH SIZES. C / REP Double dipping can sometimes be used to hot dip galvanize fabrications that are too long or wide for single immersion. If the fabrication exceeds the bath size, members in the fabrication may require touching up. Touch up and repair can be avoided, the cost of hot dip galvanizing reduced and the overall quality improved, if the design of the component is restricted to the length, width and depth of the galvanizing bath. D/B 10 DISCOLOURATION A AFTER HOT DIP GALVANIZING CAUSED BY GRINDING OR OTHER RESIDUES. C If possible Material stored in contact with rusty steel, or iron filings can cause surface rust staining. Once the cause has been removed the stains will gradually disappear. B HDGASA © 2005 9
12. 12. SC DESCRIPTION CAUSE EFFECT / REMEDY A/R/N EXAMPLE RESPONSIBILITY C/REP 11 DISTORTION. A / N The hot dip galvanizing process occurs at a molten zinc temperature of 450 deg C. This is at the lower end of the stress relieving temperature for treating steel. Thus, any inherent rolling or welding stresses in the fabrication, are likely to be released. This may result in a dimensional change, i.e. distortion. Distortion is the unwanted warping that occasionally becomes evident after hot dip galvanizing REP If Use symmetrical designs; Use sections of similar thickness; Stiffen unsupported thin wall sections; Use preformed mem-bers with the correct minimum bend radii; Use balanced or staggered weld-ing techniques; Make use of tempo-rary braces on thin walled sections such as troughs, cylinders and angle frames. Avoid quenching after galvanizing. Components can be straightened after hot dip galvanizing. D/G possible The edge most likely to have these spikes is the last to leave the bath on withdrawal. This applies particularly to complex fabrications. Drainage spikes are easily removed at the bath while still molten but with complex fabrications, the solidified spikes will be removed by fettling by the galvanizer prior to inspection. 12 DRAINAGE SPIKES. A / N Spikes and teardrops of zinc often appear along the edge of a component after hot dip galvanizing. C / REP If possible G This appearance indicates the presence of extensive iron/zinc alloy phase growth, caused by steels with high reactive levels of Silicon and Phosphorous in steels. Although not as aesthetically pleasing as a coating with free zinc on the surface, a dull grey coating provides similar or better corrosion protection. 13 DULL GREY OR A MOTTLED COATING APPEARANCE. Dull grey or mottled coatings can appear as a dark grey circular patter, a localised dull patch or, may extend over the entire surface of the component. D/S 14 ENTRAPMENT OF ASH. REP Inadequate skimming of ash from the molten zinc surface prior to dipping. On removal of ash, small uncoated surfaces shall be repaired according to the requirements of SANS 121 / ISO 1461. Large defects are a cause for rejection and require stripping and re-galvanizing. Ash which has not been (if small removed from the surface uncoated of the molten zinc prior to area immersion of steel can be R trapped on the steel (if large, surface as it is immersed negotiable) and result in an uncoated surface beneath the trapped ash. G 15 FLAKING OR R / N DELAMINATION OF COATING No adhesion of zinc to steel surface. Thick, rough coating. High phosphorous content (greater) than 0,03% causes entire coating to delaminate from the steel. Use a steel that has a phosphorous content of lower than 0,03%. D / S 16 FLUX DEPOSITS, STAINS A Flux deposits or stains may occur as a result of excessive dusting with ammonium chloride on withdrawal from the molten zinc. Flux inclusions can occur when a surface flux blanket is applied to the zinc surface (wet galvanizing). Flux blankets are normally only used for specialised processes, e.g. galvanizing of tubes and fasteners. Flux deposits or stains should be removed and the underlying coating measured to determine whether it conforms to the minimum requirements of the specification. AND INCLUSIONS Flux deposits or stains from the galvanizing process may adhere to the steel or become included in the coating. Flux residues are black, brown, grey or yellowish non-metallic C / REP deposits consisting mainly If of ammonium chloride. G necessary 10 HDGASA © 2005
13. 13. SC DESCRIPTION CAUSE EFFECT / REMEDY A/R/N EXAMPLE Inadequate repair of a damaged surface on the hot dip galvanized coating prior to the application of a paint coating. RESPONSIBILITY C/REP Make use of the correct repair materials and application procedures when touching up cut or welded hot dip galvanized components. See Coating Repair Procedures. B R REP No matter how the zinc coating is applied, the coating life is proportional to its thickness in a given environment. Often electroplated fasteners with insufficient coating thickness are incorrectly used in external environments. The use of chains, wire ropes, dragging or dropping of the component onto a hard surface, can cause mechanical damage. This is particularly relevant with thick brittle coatings. Specify hot dip galvanized fasteners to SANS 121 / ISO 1461, where required. Alternatively overcoat fastener with an approved zinc rich paint or epoxy. See Coating Repair Procedures. D / B Warning labels, highlighting a thick coating and possible damage if manhandled, should be attached by the galvanizer, before the component is transported. The use of nylon lifting slings is recommended. 19 MECHANICAL DAMAGE. A G / B Due to the shape and / or drainage conditions of some components, the hoist crane has stopped and started upon withdrawal of the items from the molten zinc. 20 OXIDE LINES. A Dross pimples result from agitation of the dross layer at the bottom of the bath or from dragging material through the dross layer. They appear as small, hard lumps on an otherwise normal galvanized surface. Blisters may be formed by hydrogen, which is absorbed during pickling and diffused at galvanizing temperatures. No effect on corrosion resistance. The overall appearance becomes uniform in time. G The galvanizer should avoid disturbing the dross layer at the bottom of the bath,by controlling immersion depth and drossing regularly. Since dross pimples represent minor disturbances in coating uniformity, they do not affect corrosion resistance. 21 PIMPLES OR BLISTERS. A G This difference in coating thickness, is brought about by a combination of a more reactive silicon killed steel, and/or high phosphorous resulting in a thicker coating and a less reactive aluminium killed steel, resulting in a coating thickness sometimes below that required in the specification. Should the galvanizer be asked to regalvanize in accordance with the specification, the resultant coating thickness on the reactive steel will be excessively thick, resulting in a brittle coating more susceptible to damage. Select the same steel for fabricating a component. If need be, accept a concession request by the galvanizer, when the thinner coating is possibly below specification. D / B R REP If accep-table REP If necessary C If necessary A / N Accept Con-cession Request 17 DISCOLOURATION OF THE PAINT COATING OVER HOT DIP GALVANIZING AFTER EXPOSURE TO THE ENVIRONMENT 18 COATING THICKNESS PROVIDED ON FASTENERS USED TO ASSEMBLE HOT DIP GALVANIZED STRUCTURES Mechanical handling or transport damage can occur, particularly with extremely thick coatings, which tend to be brittle in nature. Light aluminium oxide film lines on a hot dip galvanized surface. Pimples or blisters formed during hot dip galvanizing are usually associated with surface imperfections such as dross inclusions. 22 REACTIVE AND NON-REACTIVE STEELS, WELDED TOGETHER. Variations in coating thicknesses can arise when reactive and non-reactive steels are welded together. Efforts to increase coating thickness on the less reactive steel may result in an undesirably thick and brittle coating on the most reactive steel. HDGASA © 2005 11
14. 14. SC DESCRIPTION CAUSE EFFECT / REMEDY A/R/N EXAMPLE RESPONSIBILITY C/REP 23 REMOVAL OF ZINC R The affected areas usually only appear after the component is installed. Care should be exercised by the galvanizer to avoid over cleaning. COATING BY EXCESSIVE CLEANING Unless otherwise agreed, the galvanizer will limit cleaning of REP the final coating by At the mechanical means to galvanizer that required in the or specification. alterna-tively G / B Surface flaws in the base material may be removed by local grinding after hot dip galvanizing followed by repair of the affected surface. Minor surface defects will not adversely influence coating life. The rougher surface will produce a thicker coating and result in a longer service life. S S Excessive cleaning of the coating, particularly the edges, by mechanical methods,can result in uncoated areas. Steel may occasionally include laminations, laps, folds and non-metallic impurities, which result in slivers rolled into the metal surface. Defects of this type are sometimes detected before or after pickling, but may only become apparent after hot dip galvanizing. Rough surfaces, typical of coatings on corroded steel surfaces, can be hot dip galvanized satisfactorily. The coating will, however, reflect the texture of the substrate. Other causes of rough surfaces include uneven cold working, overpickling, a high galvanizing temperature and / or extended immersion in the molten zinc. The thicker coating produced will provide greater corrosion protection. Except when the coating tends to flake off or delaminate see SC 15. S Rough, heavy coatings refer to hot dip galvanized components showing markedly rough surfaces. This can include coatings that have a generally rough surface and, in some cases, groove type surface configurations, “tree bark effect” caused by variations in surface steel analysis. Provided the steel / casting surface is reasonably smooth, correctly centrifuged articles will provide an acceptable finish. G Efficient centrifuging, will generally remove excess zinc and provide a smooth and attractive exterior. The stains can be easily removed by means of bristle brushing. Should the component be destined for a corrosive area, the crevice should be sealed with a sealant after cleaning. D/B The salts from acid or flux that have penetrated porous welding or between contact surfaces during pickling can weep after hot dip galvanizing and water quenching, producing a stained area. at site A REP If necessary A A / R R C / REP If accept-able A C / REP If necessary 24 ROLLING DEFECTS IN STEEL. These defects may be broadly classified as surface discontinuities in the steel that have been elongated during rolling. 25 ROUGH COATINGS, CAUSED BY STEEL SURFACE CONDITIONS 26 ROUGH HEAVY COATINGS, CAUSED BY A ROUGH SURFACE AND / OR THE CHEMICAL COMPOSITION OF THE STEEL. “TREE BARK EFFECT” 27 ROUGH HEAVY COATINGS CAUSED BY INSUFFICIENT CENTRIFUGING 28 STAINS CAUSED BY WEEPING. 12 HDGASA © 2005
15. 15. SC DESCRIPTION CAUSE EFFECT / REMEDY A/R/N EXAMPLE RESPONSIBILITY C/REP The galvanizer should ensure all zinc has been removed from the inside of the pipe by longer immersion times. Minimise contact between components and jig connections. (Loosen jigging wire). Small components can be centrifuged. R C / REP If accept-able A REP If necessary and accept-able G Heavy walls and thick flanges used in the manufacture of piping can act as a heat sink when immersed in molten zinc. This effect considerably lengthens the immersion time. Occasionally the galvanizer will remove the pipes before all the zinc has melted from the inside of the pipe. Surface appearances may vary Small additions of aluminium to the A according to the chemical molten zinc, brightens the coating. composition of the steel. Cooling rate has a direct effect on the surface brightness and spangle size. Faster cooling usually results in a brighter coating with a smaller spangle size. S / G Although not particularly attractive, this condition does not adversely affect coating performance. Protuberances and lumps, which interfere with mating surfaces are unacceptable. Ensure all paint or grease is removed prior to hot dip galvanizing. Make use of suitable marking pens for temporary identification. Correctly position adequately sized vent holes. G G B Articles entering the galvanizing bath should not be in tight contact with each other. Jigging wire should also be loosely attached to eliminate wire marks. Where a component has been resting on jigging or dipping equipment, an uncoated area or touch mark could appear. This condition can occur over the entire surface or in isolated areas. Uneven drainage also includes drips on the ends of parts, runs near holes. The cause is withdrawal speed too high or low galvanizing temperature. Residues, such as oil based paint, grease, oil or labels on the steel surface or incorrectly positioned vent holes, can result in localised ungalvanized areas in an otherwise continuous galvanized coating. Defects after galvanizing can vary in colour from grey black to brown while no galvanized coating has been formed. 29 TIGHTLY ADHERENT LUMPS OF ZINC ON THE INSIDE OF HEAVY WALLED STEEL PIPING 30 TOUCH MARKS. The zinc in the galvanizing bath should have free access to all component surfaces or small uncoated or damaged areas can result. 31 TYPICAL SPANGLED HOT DIP GALVANIZED COATING. A typical hot dip galvanized surface is shown in the example. The surface is silver grey in colour and not necessary but often has a spangled effect (zinc crystals) in a range of sizes. 32 UNEVEN DRAINAGE. Uneven drainage results in an uneven or lumpy area on which zinc build up has occurred. 33 UNCOATED SURFACES CAUSED BY STEEL SURFACE CONTAMINANTS OR ENTRAPPED AIR. A C If necessary A / N / R REP If necessary These ungalvanized areas may occur in a linear pattern on angles, channels or other rolled products. They can also appear on cast iron products. S / G Sand on cast iron or scale on the steel surface is generally caused by the process used to form or roll the product. A localised ungalvanized area in an otherwise continuous coating can occur if scale or sand from the moulding or rolling is not removed by acid pickling or abrasive blasting. 34 UNGALVANIZED SURFACES CAUSED BY SCALE OR SAND. R / N REP If accept-able HDGASA © 2005 13
17. 17. Reference Areas The number and position of refer-ence areas and their sizes for the electro-magnetic test method shall be chosen with regard to the shape, varying material thick-ness and size of the article/s in order to obtain a result as repre-sentative as possible. The number of reference areas, dependant upon the size of the individual articles in the control sample, shall be as follows: a) For articles with significant surfaceB area greater than 2m2, at least three reference areas shall be taken on each control sample. b) For articles with a total signif-icant surface area greater than 2m2, manufactured from material of several different thickness’, at least three ref-erence areas shall be taken on each specific material thickness. c) For articles with signifi-cant surface area between 1 000mm2 and up to and in-cluding 2m2 inclusive, each article in the control sample shall have at least one refer-ence area. d) For articles with a total signif-icant surface area between 1 000mm2 and up to and including 2m2 inclusive, man-ufactured from material of several different thickness’, each different material thick-ness, representing the con-trol sample shall have at least one reference area, per mate-rial thickness. e) For articles with less than 1 000mm2 of significant sur-face area, enough articles shall be grouped together to pro-vide at least 1 000mm2 surface for an individual reference area. The number of reference areas shall be as given in the last column of table 1. Hence, the total number of articles tested equals the number of articles required to provide one reference area multiplied by the appropriate number from the last column of table 1 related to the size of the lot (or the total number of articles galvanized if that is less). Alternatively, sampling pro-cedures selected from SANS 2859-1 / ISO 2859-1shall be used. Note: 2m2 is typically 200 cm x 100 cm and 1 000 mm2 is typically 10 cm x 1 cm. For case a) and b) on each article taken separately in the control sample, the local coating thick-ness within the reference area shall be equal to or greater than the mean coating thickness val-ues given in table 2 or 3 or the local coating thickness values given in table 4. In cases c) to e) the coating thick-ness on each reference area shall be equal to or greater than the local coating thickness values given in table 2, 3 or 4 as appro-priate. The mean coating thick-ness on all reference areas on material of equal thickness in a sample shall be equal to or greater than the mean coating thickness values given in table 2 or 3 as appropriate. When more than five articles have to be taken to make up a reference area of at least 1 000 mm2, a single magnetic measurement shall be taken on each article if a suitable area of sig-nificant surface exists: if not, the gravimetric test shall be used. Within each reference area, which should be at least 1 000 mm2, a minimum of five magnetic test readings shall be taken. If any of the individual readings is lower than the values in table 2 or 3, this is irrelevant as only the mean value over the whole of each reference area is required to be equal to or greater than the local thickness given in the table. Thickness measurements shall not be taken on cut surfaces or areas less than 10mm from edges, flame cut surfaces or corners. Uniformity Testing Variations in coating thickness are not usually of concern with materials hot dip galvanized after fabrication provided the minimum coating thickness requirements are satisfied, (except for fasteners - see note on maximum coating thickness below table 3.) Where the coat-ing thickness is not uniform, the service life of the galvanized coating will generally be gov-erned by the amount of zinc available at the place where the coating is thinnest rather than by the overall or average thickness of the coating. Standard magnetic measuring instruments are quick and conve-nient methods for determining local coating thickness. By tak-ing a number of readings on a hot dip galvanized surface, uni-formity as well as actual thick-ness can be easily checked. If small specimens are available, it may be possible to use the Preece test as a measure of coat-ing uniformity. This test pro-vides limited information as to the coating thickness, but serves only to locate the thinnest spot in a zinc coating by chemically removing the zinc. There are many limitations on the use of the Preece test; con-sequently, it is no longer referred to in specifications for B A significant surface can be defined as a surface which impacts on the performance of that article. HDGASA © 2005 15
19. 19. galvanized articles may require the use of chain slings, wire or other holding devices to immerse the material into the galvanizing bath if suitable lifting fixtures are not pro-vided on the item. Chains, wire and special jigs used to handle the items may leave a mark on the hot dip galvanized item. These marks are not always detrimental and reason for rejection. Should these marks, be greater than 5mm2 per chain mark and expose the bare steel, suitable repair should be car-ried out using the procedures indi-cated in SANS 121 / ISO 1461. See also “Coating Repair Procedures”. Differences in the lustre and colour of hot dip galvanized coat-ings do not affect corrosion resis-tance and the presence or absence of spangle has no effect on coating performance. The well-known spangled effect found on some hot dip galva-nized surfaces is simply a factor of primary crystallisation. It is chiefly dependant upon the zinc bath chemistry, the rate of cool-ing, the method of pickling, the steel chemistry, and the thickness of the coating. In fact, dull grey or patchy matte grey hot dip gal-vanized coatings give service lives equal to or greater than bright or spangled coatings. Variations in coating appearance or finish are important only to the extent that they will affect corro-sion performance or the intended use of the article. The primary function of a hot dip galvanized coating is corrosion protection. Specific requirements beyond the standard set out in SANS 121 / ISO 1461, shall be communicat-ed to the galvanizer in writing or discussed at the contract review, prior to the work being hot dip galvanized. The information supplied may include – a) The composition and any properties of the metal that may affect the quality of the hot dip galvanized coating. b) Identification of significant surfaces. See page 15B for definition. c) A visual standard should be established if a special finish is required. d) Any particular treatments that are required or not required before or after the process. e) A variance in coating thick-ness. See notes below table 3. f) The acceptable method of repair, if this is found to be necessary – see also “Coating Repair Procedures” Removal of Wet Storage Stain (White Rust) Although in extreme cases the protective value of the coating may be impaired, wet storage stain attack is often superficial despite the relative bulkiness of the corrosion product. Where surface staining is light and smooth without growth of the zinc oxide layer as judged by lightly rubbing fingertips across the surface, the staining will gradually disappear and blend in with the surrounding zinc surface as a result of normal weathering in service. When the affected area will not be fully exposed in service or when it will be subjected to a humid environment, wet storage staining must be removed, even if it is superficial. This is essential for the basic zinc carbonate film to form. The formation of this zinc carbonate film is necessary to ensure long term service life. Light deposits can be removed by cleaning with a stiff bristle (not wire) brush. Heavier deposits can be removed by brushing with a 5% solution of sodium or potassi-um dichromate with the addition of 0.1% by volume of concentrat-ed sulphuric acid. Alternatively, a 10% solution of acetic acid can be used. These solutions are applied with a stiff brush and left for about 30 seconds before thoroughly rinsing and drying. Unless present prior to shipment from the galvanizer, the develop-ment of wet storage stain is not the responsibility of the galvaniz-er. The customer must exercise proper caution during trans-portation and storage to protect against wet storage staining. Coating Repair Procedures BY THE GALVANIZER In terms of SANS 121 / ISO 1461 a galvanizer may repair a coating by either zinc metal spraying or zinc rich epoxy or paint. The latter method must conform to certain requirements in the specification. The pre-ferred method of repair is by zinc metal spraying. Repair will only be necessary if bare spots are present, usually caused by inadequate cleaning, air entrap-ment or if mechanical damage has occurred. The total uncoated areas for ren-ovation by the galvanizer shall not exceed 0,5% of the total area of the component. For articles equal to an area of 2m2; 0,5% represents a maxi-mum area of 100cm2 or 100mm x 100mm. For articles equal to an area of 10 000mm2; 0,5% represents a maximum area of 50mm2 or 7mm x 7mm. No individual repair area shall exceed 10cm2 or 10mm x 100mm. If uncoated areas are greater than 0,5%, the article shall be HDGASA © 2005 17
20. 20. regalvanized, unless otherwise agreed between the purchaser and the galvanizer. Zinc Metal Thermal Sprayed Coatings Method The damaged area is to be lightly blasted using preferably a pencil blasting nozzle or the surround-ing coating should be masked in order to limit damage. A zinc metal sprayed coating is then applied to the abrasively blasted surface to a thickness at least 30μm greater than the minimum specified zinc coating thickness, or equal to the sur-rounding coating thickness, whichever is the greater. The repaired area is then wire brushed (preferably stainless steel) to remove loosely adher-ing over sprayed zinc. Wire brushing provides the added benefit of sealing the pores that may be present in the sprayed coating. Zinc Rich Epoxy or Zinc Rich Paint Method The defective area shall be blast-ed as above or abraded with abrasive paper (roughness 80 grit). All dust and debris must be completely removed. In the event of moisture being pre-sent, all surfaces are to be prop-erly dried. A zinc rich paint or epoxy con-taining not less than 80% of zinc in the dry film (53% by volume), should be applied to a thick-ness, 30μm greater than the minimum specified for the gal-vanized coating or equal to that of the surrounding galvanized coating, whichever is greater. The paint coating should over-lap the surrounding zinc by at least 25mm. The preferred product is a two or three component zinc rich epoxy. SITE REPAIRS The preferred method of repair is by zinc metal thermal spraying. Due to the remoteness of most sites, however, and the unavail-ability of metal spraying equip-ment, repairs by zinc rich epoxy or zinc rich paint have to date generally been more popular. Site repairs should be limited to small coating defects and areas that have been cut or welded on site. Should excessive amounts of grease or oil be present at the affected area, it should be removed by means of an approved solvent. All residues are to be thoroughly removed by washing with clean water. The affected area should then be abraded with abrasive paper (roughness 80 grit) or alterna-tively thoroughly cleaned using, preferably a stainless steel brush. All dust and debris should be completely removed. Repair can now be carried out using an approved product. Single pack zinc rich paints are good materials and can easily be applied. They, however, require several coats to achieve a rea-sonable repair. Multiple coats will also necessitate longer dry-ing times between coats. Site Repairs by “Zincfix” Until recently, the approved products for repair were only available in large containers. Due to the large quantities involved and short pot life when mixed, the products proved to be expensive and wasteful. A product is now available in a three component, solvent free form, packed for convenience in handy, easy to use squish packs. The repair product is called “Zincfix” and is approved by and available from the Hot Dip Galvanizers Association of Southern Africa and all of its members. The product has been tested against a number of reputable products and has performed exceptionally well. Zincfix is available in a 100g squish pack and will coat an area of about 0,25m2 to a DFT (Dry film thickness) of 100 to 150μm in a single application. The contents are easily mixed in accurate proportions. 18 HDGASA © 2005
21. 21. APPENDIX A Applicable Standards SANS 121 / ISO 1461 Hot dip galvanized coatings on fabricated iron HDGASA © 2005 and steel articles - Specifications and test methods SABS 763 Hot dip (galvanized) zinc coatings (other than on continuously zinc coated sheet and wire). SANS 32 / EN 10240 Internal and/or external protective coatings for steel tubes – Specification for hot dip galva-nized coatings applied in automatic plants. SANS 14713 / ISO 14713 Protection against corrosion of iron and steel in structures – Zinc and aluminium coatings – Guidelines. SANS 2178 / ISO 2178 Non-magnetic coatings on magnetic substrates - Measurement of coating thickness – Magnetic method. ISO 1460 Metallic coatings – Hot dip galvanized coatings on ferrous materials – Gravimetric determina-tion of the mass per unit area. SANS 8492 / ISO 8492 Metallic materials – Tube – Flattening test. The Hot Dip Galvanizers Association of Southern Africa is indebted to the American Galvanizers Association and Industrial Galvanizers Corporation (Pty) Ltd of Australia, for permission to include some of the contents of their publication on inspection after hot dip galvanizing. 19
22. 22. HDGASA © 2005 The Hot Dip Galvanizers Association of Southern Africa Introduction: The Hot Dip Galvanizers Association of Southern Africa was founded in 1965 and its membership represents over 90% of the available hot dip galvanizing capacity of Southern Africa. The Vision: To position the Hot Dip Galvanizers Association of Southern Africa, comprising all its Members and other interested parties, as a professional organization serving the interests of all parties dependant upon the hot dip galvanizing industry. Mission Statement: To develop and expand the demand for hot dip galvanizing, identify and develop new market opportunities for the benefit of Members and other stakeholders. Strategic Objective: To convince users and specifiers to use hot dip galvanized steel in preference to other coatings and alternative materials, where suitable. This is carried out in three ways: 1. Through the use of general promotion activities. 2. Through focused technical marketing support. 3. Through training and education programmes. Delivery Activities: Promoting the use of hot dip galvanizing for cost effective corrosion protection in applications where its use is appropriate. Providing technical assistance and advice for specifiers, fabricators and end users while also recommending alternative protective methods where appropriate. Identifying and investigating potential new applications for hot dip galvanizing. Participating in development projects on behalf of industry by providing assistance in the form of technical consulting, practical recommendations and assistance with the preparation of design specifications. Providing assistance with quality control during fabrication and hot dip galvanizing. Disseminating technical knowledge by providing a consulting and training service as well as the publication of technical literature. Providing training and education for member companies to ensure a high standard of quality and service throughout the hot dip galvanizing industry. 20 Publications Available from the Association Steel Protection by Hot Dip Galvanizing and Duplex Systems. Practical Guidelines for the Inspection and Repair of Hot Dip Galvanized Coatings. Specification for the Performance Requirements of Duplex Coating Systems. Code of Practice for Surface Preparation and Application of Organic Coatings Applied to New Unweathered Hot Dip Galvanized Steel. Guidelines for the Use of Hot Dip Galvanized Products in the Mining Industry. Wall Chart - Design for Hot Dip Galvanizing. Hot Dip Galvanizing Industry Buyers’ Guide. HOT DIP GALVANIZING HAS BEEN USED TO PROTECT STEEL FROM CORROSION FOR MORE THAN 160 YEARS. APPLICATIONS FOR WHICH HOT DIP GALVANIZING IS SUITABLE ARE NUMEROUS AND VARIED AND THE DEMAND CONTINUES TO INCREASE.
23. 23. RELIABILITY The hot dip galvanized coating is formed by a metallurgical reaction between suitably cleaned steel and molten zinc. This results in the formation of a series of iron/zinc alloys which are overcoated with relatively pure zinc. The process entails total immersion of components in both pretreatment chemicals and molten zinc. This ensures uniform protection and coating reliability even on surfaces which would be inaccessible for coating by other methods. DEPENDABILITY Ease of inspection and dependability in service are beneficial features of a hot dip galvanized coating. The cathodic protection of steel by zinc ensures that corrosion of the underlying steel cannot occur as long as zinc is present. Even at discontinuities on the coating, corrosion creep under the surrounding zinc is not possible. PREDICTABILITY The durability of a hot dip galvanized coating is determined by the degree of corrosion of zinc in a specific environment and the thickness of the coating. Corrosion of zinc is normally uniform, thus durability of a hot dip galvanized coating is predictable in most applications. ISSUE DATE: NOVEMBER 2005